See discussions, stats, and author profiles for this publication at: https://www.researchgate.net/publication/257497932 Crack width evaluation for ﬂexural RC members Article in AEJ - Alexandria Engineering Journal · September 2012 DOI: 10.1016/j.aej.2012.05.001 CITATIONS READS 13 1,234 4 authors, including: Said M. Allam Mohie S. Shoukry Facultry of Engineering, Alexandria University Alexandria University 13 PUBLICATIONS 158 CITATIONS 9 PUBLICATIONS 42 CITATIONS SEE PROFILE All content following this page was uploaded by Said M. Allam on 01 December 2014. The user has requested enhancement of the downloaded file. SEE PROFILE Alexandria Engineering Journal (2012) 51, 211–220 Alexandria University Alexandria Engineering Journal www.elsevier.com/locate/aej www.sciencedirect.com ORIGINAL ARTICLE Crack width evaluation for ﬂexural RC members Said M. Allam *, Mohie S. Shoukry, Gehad E. Rashad, Amal S. Hassan Structural Engineering Department, Faculty of Engineering, Alexandria University, Alexandria, Egypt Received 18 February 2012; revised 8 May 2012; accepted 9 May 2012 Available online 20 July 2012 KEYWORDS Flexural cracks; Crack width; Cover; Serviceability; Reinforced concrete; Codes provisions Abstract Some building code equations and equations developed by researchers are used for the calculation of the crack width in reinforced concrete ﬂexural members. To investigate codes’ provisions beside some equations found in the literature concerning the crack width calculation of reinforced concrete members subjected to ﬂexure, ﬁve reinforced concrete rectangular models were investigated theoretically. The models include different parameters such as reinforcement steel ratio, steel rebar arrangement and reinforcement grade. Also, to verify the accuracy of the building code equations and the equations developed by researchers a comparison against some experimental data available in the literature was carried out. The experimental data include some variables affecting the crack width such as steel stress, concrete cover, ﬂexural reinforcement ratio and rebar arrangement. The study showed a large scatter among the different code equations, however, most of the code equations overestimate the effect of concrete cover on the calculated values of the crack width. Also, the Egyptian code equation should limit the value of the mean steel stress as given by Eurocode equation to overcome the underestimated values obtained in the case of sections having low steel ratio. Moreover, the reinforcement detailing (bars distribution) is an important factor affecting the crack width. ª 2012 Faculty of Engineering, Alexandria University. Production and hosting by Elsevier B.V. All rights reserved. 1. Introduction Crack width calculation is one of the serviceability requirements in the structural concrete elements. The occurrence of cracks in reinforced concrete elements is expected under service loads, due to the low tensile strength of concrete. Control of * Corresponding author. Tel.: +20 01112244066. E-mail address: [email protected] Peer review under responsibility of Faculty of Engineering Alexandria University. Production and hosting by Elsevier cracking is important for obtaining acceptable appearance and for long-term durability of concrete structures, especially those subjected to aggressive environments. Excessive crack width may reduce the service life of the structure by permitting more rapid penetration of corrosive factors such as high humidity, repeated saturation with moisture, vapor, salt-water spray and gases with chemicals, to reach the reinforcement. Generally, cracking should not induce reinforcement steel corrosion or spoil the appearance of the structure. In addition, cracking in reinforced concrete structures has an effect on structural performance including stiffness, energy absorption, capacity, and ductility. Consequently, there is an increased interest in the control of cracking by building codes and scientiﬁc organizations. With the use of ultimate strength 1110-0168 ª 2012 Faculty of Engineering, Alexandria University. Production and hosting by Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.aej.2012.05.001 212 S.M. Allam et al. methodology and high strength reinforcement steel, researchers and designers recognized the need for providing a mechanism by which crack width would be minimized. Therefore, researches were undertaken in 1960s to quantify the above concept and develop design tools . The crack width of a ﬂexural member is obtained by multiplying the maximum crack spacing by the mean strain of the ﬂexural steel reinforcement. Therefore, the crack width depends on the nature and the arrangement of the reinforcing steel crossing the cracks and the bond between the steel bars found in the tension zone of concrete. Many research work found in the literature predicted the crack width of a ﬂexural member based on theoretical models and experimental data. Saliger  and Tomas  used Bond-Slip model, Borms  and Base et al.  used No-Slip model, however Welch and Janjua  and Leonhardt  used Localized Bond-Slip model to predict the crack width. Gergely and Lutz  used the results of experimental data to formulate an equation to calculate the crack width. Based on the experimental work, Oh and Kang  proposed a formulation for predicting the maximum crack width. Frosch  developed a simple theoretical equation to predict the crack width based on a physical model. Besides the research work carried out for crack width formulation, other research work experimentally investigated the factors affecting the crack width. Makhlouf and Malhas  investigated the effect of thick concrete cover on the maximum ﬂexural crack width under service load. Beeby  and Nawy and Blair  showed that the transverse reinforcement had a strong inﬂuence on the crack spacing. Gilbert and Nejadi  tested six beams and six one-way slabs with different ﬂexural reinforcement ratio and bar arrangement including various concrete cover. In this paper, a study is carried out to investigate several formulas suggested by different building codes for the calculation of the crack width in reinforced concrete ﬂexural members. Also, the formulas proposed by other researchers were also investigated and compared with codes’ equations. In addition, the most prevalent building codes’ equations are examined and tested against some experimental data available in the literature. Moreover, a comparison was carried out among the equations to discuss the various factors and parameters affecting the crack width. 2. Crack width prediction according to some building codes provisions 2.1. Eurocode2 1992-1 (2001) Eurocode2  gives the following equation for predicting the crack width of ﬂexural members Wk ¼ Sr;max ðesm ecm Þ ð1Þ where Wk = the design crack width, mm. The mean tensile strain esm ecm) is given by the following equation: eff Þ fs Kt fcteff ð1þnq qeff fs P 0:6 ð2Þ ðesm ecm Þ ¼ Es Es where esm is the mean strain in the reinforcement under the relevant combination of loads, including the effect of imposed deformations and taking into account the effects of tensioning stiffening. Only the additional tensile strain beyond zero strain in the concrete is considered; ecm is the mean strain in concrete between cracks. Kt = factor expressing the duration of loading: Kt = 0.6 for short term loading and Kt = 0.4 for long term loading, fs = the stress in the tension reinforcement computed on the basis of a cracked section, n = the modular ratio Es ; fcteff = the mean value of tensile strength of the concrete Ecm effective at the time when the cracks may ﬁrst be expected to occur, qeff ¼ As Aceff Aceff = effective tension area, is the area of concrete surrounding the tension reinforcement. Sr,max = the maximum crack spacing, mm and is given by the following equation Sr;max ¼ 3:4c þ 0:425k1 k2 /=qeff ð3Þ where c = concrete clear cover, k1 = coefﬁcient that takes into account the bond properties of the bonded reinforcement and equals to 0.8 for high bond reinforcing bars, and equals to 1.6 for plain reinforcing bars, / = the bar diameter, mm; in case of using various diameters, the average diameter shall be used, k2 = coefﬁcient that takes into account the strain distribution and is equal to 0.5 for sections subjected to pure bending and equals to 1.0 for sections subjected to pure axial tension. 2.2. Egyptian code; ECP 203-2007 The Egyptian code ECP 203-2007  gives the crack width by the following equation: Wk ¼ besm Srm ð4Þ where Wk = coefﬁcient for checking crack width condition, mm; Srm = average stabilized crack spacing, mm; esm = mean steel strain under relevant combination of loads and allowing for the effect such as tension stiffening or shrinkage; b = coefﬁcient relating the average crack width to the design value: b = 1.7 for cracks induced by loading and for cracking induced by restraining the deformation for cross section having width or depth (whichever smaller) in excess of 800 mm, and b = 1.3 for cracking induced by restraining the deformation for cross section having width or depth (whichever smaller) less than 300 mm. The mean steel strain esm is given as 2 ! fs fscr2 esm ¼ 1 b1 b2 ð5Þ Es fs where fs = stress in the tension reinforcement calculated on the basis of a cracked section, N/mm2; fscr2 = stress in the tension longitudinal reinforcement computed on the basis of a cracked section under loading conditions that cause the ﬁrst crack, N/mm2; b1 = a coefﬁcient accounting for bar bond characteristics, and is equal to 0.8 for deformed bars and 0.5 for plain smooth bars, b2 = a coefﬁcient accounting for load duration; is equal to 1.0 for single short-term loading and 0.5 for sustained or cyclic loading; Es = Modulus of elasticity of the reinforcement, N/mm2. The Egyptian code gives the average stabilized mean crack spacing by the following equation: Srm ¼ 50 þ 0:25k1 k2 /=qeff ð6Þ Crack width evaluation for ﬂexural RC members 213 However, the items of the above equation are similar to the items of the equation given by the Eurocode2  with the assumption that the clear concrete cover is equal to 25 mm. 2.4. British standards BS 8110-1997 According to BS 8110-1997 , the width of ﬂexural cracks at a particular point on the surface of a member depends primarily on three factors: 2.3. ACI 318 Prior to 1999, ﬂexural crack control requirements in ACI were based on the so-called z-factor method developed be Gergely and Lutz . Their work was based on extensive statistical analysis techniques on experimental data from several researchers. The equation proposed by the early version of ACI 318-95  took the following form: pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Wmax ¼ 0:011bfs 3 dc Ao 103 mm; ð7Þ where b ¼ hx is the ratio of distance between neutral axis dx and extreme tension face to distance between neutral axis and centroid of reinforcing steel; b = 1.20 in beams may be used to compare the crack widths obtained in ﬂexure and axial tension. Ao = the area of concrete surrounding each reinforcing bar = Ae/nb, Ae = the effective area of concrete in tension, Ae can be deﬁned as the area of concrete having the full width of the beam and having the same centroid of the main reinforcement; Ae = 2 dcb, nb = the number of tension reinforcing bars. dc = the distance measured from the centroid of tensile steel to the extreme tensioned ﬁber The ﬂexural crack width expression in the above equation, with hx ¼ 1:2 , is used in ACI 318-95 in the following form: dx p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 z ¼ fs dc Ao ð8Þ A maximum value of z = 3064.5 N/mm is permitted for interior exposure, corresponding to a limiting crack width of 0.41 mm. ACI 318-95 also limits the value of z to 2539.2 N/ mm for exterior exposure, corresponding to a crack width of 0.33 mm. When structures are subjected to very aggressive exposure or designed to be watertight, ACI committee 350 , limits the value of z to 1700 N/mm corresponding to a crack width of 0.20 mm. In the 1999 edition, ACI decided to greatly simplify crack control requirements due to increased evidence suggesting a reduced correlation between crack width and reinforcement corrosion. Beeby  and  showed that corrosion does not correlate with surface crack widths in the range normally found with reinforcement stresses at service load levels. Therefore, ACI introduced changes to the crack rules in which a maximum bar spacing, rather than a z-factor (related to crack width) is prescribed. ACI 318-05 , ACI 31808  proposed the following equation for crack control: s ¼ 380ð280=fs Þ 2:5c 300ð280=fs Þ ð9Þ where s = maximum spacing of reinforcement closest to the tension face, mm; c = least distance from surface of reinforcement to tension face, mm. However the equation does not make a distinction between interior and exterior exposure, i.e. the exposure conditions dependence was eliminated. Also, the equation is indirectly tied to a crack width equals to 0.4 mm. The value of fs at service load shall be computed on the basis of service moment. ACI permits the use of fs = 0.67 fy. (a) The proximity to the point considered of reinforcing bars perpendicular to the cracks; concrete cover. (b) The proximity of the neutral axis to the point considered; h–x. (c) The average surface strain at the point considered. BS 8110-1997 recommends that the strain in the tension reinforcement is limited to 0.8 fy/Es (i.e. 0.8 \ steel yield strain) and the design surface crack width should not exceed the appropriate value. Cracking should not lead to spoil appearance. So for members that are visible, the calculated maximum crack width should not exceed 0.30 mm. Also, cracking should not lead to steel corrosion, so for members in aggressive environment the calculated maximum crack width should not lead to a loss of the performance of the structure. BS 8110-97 provisions are based on Beeby  empirical equations, Design surface crack width Wd ¼ 3 acr em cmin 1 þ 2 acrhx ð10Þ where acr = distance from the point considered to the surface of the nearest longitudinal bar; em = average strain at the level where the cracking is being considered; cmin = minimum cover to the tension steel; h = overall depth of the member; x = depth of neutral axis. For cracked section, the value of em is expressed as: em ¼ e1 bðh xÞða0 xÞ 3Es As ðd xÞ ð11Þ where e1 = strain at the level considered, calculated ignoring the stiffening effect of the concrete in the tension zone, b = width of the section at the centroid of the tension steel, a0 = distance from the compression face to the point at which the crack width is being calculated. According to BS 8110-1997 , in assessing the strains, the modulus of elasticity of the concrete should be taken as half the instantaneous values. 3. Some signiﬁcant formulas for crack width given by researchers 3.1. Gergely and Lutz Gergely and Lutz  used test results from Hognestad , Kaar and Mattock , Kaar and Hognestad , Clark , and Rusch and Rehm , to conclude their equation for the calculation of crack widths at the tension surface. As stated by Frosch , the maximum concrete cover; dc used in the tests analyzed by Gergely and Lutz  was 84 mm and only three specimens of 612 observations had clear covers greater than 64 mm. The original equation developed by Gergely and Lutz  is as follows: pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Ws ¼ 0:011 3 ðc þ /=2ÞAo ðfs 34:45Þ 103 ð12Þ 214 S.M. Allam et al. 1=3 t 4:5 A0 b a0 ¼ 159 þ 2:83 hx As1 ð14Þ R ¼ ðh xÞ=ðd xÞ ð15Þ where A0 is the effective area of tensioned concrete around each reinforcing bar; Ao = Ae/nb and Ae = b h1, h1 is the depth of equivalent area, ðh xÞ3 ð16Þ 3ðd xÞ2 0:236 106 Sm ¼ / c0 þ e2s ð17Þ In which, 1=3 t 4:5 Ao b þ 1:66 c0 ¼ 25:7 hx As1 4.Comparison between some code equations and other available equations for predicting the crack width of some theoretical models In this section, the above mentioned building codes and some equations given by researchers are applied to ﬁve reinforced concrete sections having different values of reinforcement ratio, bar distribution, and bars grade. Fig. 1 shows the layout of the ﬁve models. The Models 1, 2, and 3 have the same reinforcement (strength; fy, type: deformed bars, number and diameter), section width; b, concrete strength; fcu. These models varied in section depth; d and consequently have variable reinforcement ratios; l. Values of l were: 0.565%, 0.87%, and 1.21% for the three model respectively. Models 2 and 4 have identical properties (same steel reinforcement, same section dimensions) and they varied in bar surface condition and yield stress of steel. Plain mild steel bars were used for Model 4, while high strength deformed bars were used for Model 2. Models 2 and 5 have the same section dimensions, approximately, same area of tension steel but varied in bar distribution (number and diameter). The values of the crack width were calculated at the same steel stress level 332 mm 370 mm 462 mm 500 mm 5 16 30 16 30 5 38 mm 16 30 5 38 mm 712 mm 750 mm ð18Þ 250 mm 250 mm 250 mm model 1 model 2 model 3 Figure 1 2 5 16 30 h1 ¼ c 457.5 mm 500 mm In which, ð19Þ 250 mm model 4 Dimensions and reinforcement of the studied models. 2 25 30 ð13Þ fs db Es where d\ is the controlling cover distance and is taken the 8 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 9 < d2 þ d2 = c s greater of qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ; b ¼ hx and ds is the side cover. dx : d2 þ s 2 ; 38 mm Wmax ¼ /a0 ðes 0:0002ÞR Wmax ¼ 2 250 mm model 5 42.5 mm Oh and Kang  proposed a formulation for predicting the maximum crack width; Wmax and average crack spacing; S in reinforced concrete ﬂexural members. They tested ﬁve reinforced concrete beams with design variables including the concrete cover, diameter of steel bars, reinforcement ratios, spacing of steel bars and steel stress. Based on an energy approach, Oh and Kang concluded a new deﬁnition of the effective area of concrete in tension and suggested the following equation for the calculation of the maximum crack width: Frosch  stated that Eq. (7) proposed by ACI-95  is valid for a relatively narrow range of concrete covers (i.e. up to 63 mm). The use of thicker concrete covers is increasing because research and experience have indicated that the use of thicker covers can increase durability. Therefore, Frosch  developed the following simple, theoretically-derived equation to predict crack widths that could be used regardless the actual concrete cover. 462 mm 500 mm 3.2. Oh and Kang 3.3. Frosch 38 mm where Ws = the most probable maximum crack width at level of steel, mm; fs = the reinforcement steel stress, N/mm2; Ao = the area of concrete symmetric with reinforcing steel divided by number of bars, mm2. To obtain the maximum crack width at the extreme tensioned ﬁber, Eq. (12) is multiplied by a factor b ¼ hx . dx Crack width evaluation for ﬂexural RC members Table 1 215 Values of the crack width for the studied models. Equation Eurocode2 ECP-2007 ACI 318-95 BS 8110-97 Gergely and Lutz  Frosch  Oh and Kang  Crack width (mm) Model 1 Model 2 Model 3 Model 4 Model 5 0.127 0.107 0.124 0.079 0.102 0.101 0.147 0.127 0.129 0.129 0.087 0.107 0.106 0.135 0.127 0.137 0.136 0.090 0.113 0.111 0.131 0.107 0.123 0.119 0.056 0.0682 0.0742 0.0845 0.16 0.170 0.191 0.162 0.158 0.231 0.218 (fs = 200 N/mm2 for models 1, 2, 3 and 5 and fs = 140 N/mm2 for model 4). Concrete strength was considered as fcu = 30 N/ mm2 and the clear cover = 30 mm. Table 1 shows the values of crack widths calculated for the studied models for both of code equations and equations given by Gergely and Lutz , Frosch  and Oh and Kang . The following was observed concerning the results given in the Table 1: i. Generally, values of crack width predicted by the code equations showed a large scatter among the different code equations and those obtained by previous researchers. Values of crack width, predicted using BS 8110-97, were less than those predicted by other building codes or by equations developed by researchers, especially for Model 4, reinforced with plain mild steel bars. Values of the crack width predicted by the Egyptian code were very close to those predicted by ACI 318-95 and Eurocode2 equations except for model 1 with low reinforcement ratio; l. The Egyptian code equation predicts values of crack width for sections with low reinforcement ratio smaller than those predicted by ACI or Eurocode2. Also, the table indicates that the equation of Oh and Kang  overestimated the values of the crack widths in the case of low steel ratio (Model 1), however ECP-2007 overestimated the value of the crack width in the case of plain bars of model 4. ii. Comparing the results of the crack widths calculated for the models 1,2 and 3 indicated that as the percentage of the ﬂexural steel ratio, l, increased the calculated values of the crack width increased. This is given by code equations of ECP-2007, ACI-318-95 and other equations given by Gergely and Lutz  and Frosch . With the increase of l, the concrete contribution in tension decreases and the mean steel strain increases, and then the crack width consequently increases. However, according to Eurocode2, the increase of l does not affect the crack width. On contrary, the equation of Oh and Kang  is found to give low values of crack width with the increase of the ﬂexural steel ratio, l. iii. The effect of using different numbers of steel bars with equal area on the crack width is investigated by comparing the results of models 2 and 5. It is well established that the bar distribution is an important factor affecting crack width. With well choice of bar arrangement (larger number, smaller diameter), better bond between concrete and steel occurs and thus reducing the crack spacing. The reduction in crack width due to better bar distribution ranged from 26% to 118%, the lowest value was obtained using the Eurocode2 equation and the highest value was obtained according to Frosch  equation. The equation developed by Frosch  indicates that crack spacing (and consequently crack width) depends mainly on the distance between reinforcement bars. iv. The effect of bar surface condition (plain or deformed) on crack width was obtained by comparing the results of models 2 and 4. The use of plain mild steel bars (with low steel stress at service loads) results values of crack width less by about 5–56% compared with model reinforced with the same area of high strength deformed bars. The lowest value was obtained using the ECP2007 equation and the highest value was obtained by Oh and Kang equation. The effect of bar surface deformation on the calculation of crack width not only affects the crack spacing, but also affects the mean strain. When the bond between the concrete and the steel increased, more tension force is transferred to the concrete between cracks. With the increase in the concrete contribution in tension, less slip between concrete and steel occurs, hence less value of total elongation between them (esm ecm); and consequently resulting in less crack width. However, the effect of bar surface deformation is not considered in code formulas except the Egyptian code and Eurocode2. 5. Application of some code equations to some available experimental data To asses the accuracy of code equations and the most common formulas for predicting crack width in reinforced concrete members, a comparison is carried out with the experimental results reported by Makhlouf and Malhas . The comparison includes two factors affecting the crack width such as the steel stress and concrete cover. 5.1. Makhlouf and Malhas Makhlouf and Malhas  reported results of tests on 11 beams reinforced with high strength deformed bars. The maximum crack width was recorded at the reinforcement level. The specimens consisted of two groups. Group ‘‘A’’ consisted of eight beams four of them were with 22 mm concrete clear cover and the other four were with 52 mm concrete clear cover. Group ‘‘A’’ mainly intended to investigate the effect of 216 S.M. Allam et al. Figure 2 Table 2 Group ‘‘A’’ Group ‘‘B’’ Beam specimens tested by Makhlouf and Malhas . Properties of specimens tested by Makhlouf and Malhas . Specimen no. b (mm) h (mm) d (mm) Reinforcement steel Reinforcement ratio; l (%) fc0 (N/ mm2) fy (N/ mm2) c (mm) GA11 180 430 400 2Ø12 0.31 34 425 22 GA12 GA13 GAM GA21 GA22 GA23 GA24 180 180 180 180 180 180 180 430 430 430 460 460 460 460 400 400 400 400 400 400 400 2Ø16 2Ø20 2Ø25 2Ø12 2Ø16 2Ø20 2Ø25 0.56 0.87 1.36 0.31 0.56 0.87 1.36 34 34 34 34 34 34 34 425 425 425 425 425 425 425 22 22 22 52 52 52 52 Gl 600 400 338 4Ø14 + 2020 0.62 40 430 50 G2 G3 600 600 400 400 336 336 6Ø20 9Ø20 0.94 1.40 40 40 430 430 50 50 doubling the concrete clear cover on the crack width. Group ‘‘B’’ consisted of 3 wide beams of 600 mm width, 400 mm depth and clear concrete cover = 50 mm. The experimental specimens were tested under a load level of 80–110% of service load. Group ‘‘B’’ aimed to assess the magnitude of crack widths in full-size beams under different levels of steel stress. Fig. 2 shows the dimensions and loading system of the tested beams while Table 2 gives properties of all specimens tested by Makhlouf and Malhas  for both Group ‘‘A’’ and Group ‘‘B’’. Measurements were taken on both sides of the beam specimens and at 10 mm above the lower edge. Readings were taken at predetermined load levels that corresponded to a speciﬁc safety factor relative to the ultimate failure load. 5.1.1. Effect of steel stress, fs The main and the most important factor affecting the crack width is the steel strain (stress) which is directly proportional with the crack width. Makhlouf and Malhas  measured the crack width of the specimens of Group ‘‘B’’ at different levels of steel stress, as given in Table 3. Figs. 3–5 display the relationship between the crack width; Wmax, as calculated using codes’ equations, and the steel stress; fs, for the group ‘‘B’’ specimens: G1, G2, and G3 respectively. A summary of the results obtained from code’s equations is given in Table 3. From the Figures and Table the following are observed: i. The Egyptian code gives underestimated values of crack width for sections reinforced with low reinforcement ratios (l = 0.62%), especially at low levels of steel stress 0.14 0.18 0.26 0.34 0.13 0.17 0.22 0.29 0.18 0.21 0.27 0.33 pﬃﬃﬃﬃﬃﬃ Tensile strength of concrete fctr ¼ 0:6 fcu ¼ 4:12 N=mm2 , – uncracked section according to the Egyptian code. 2 Tensile strength of concrete fctm ¼ 0:3ðf0c Þ3 ¼ 3:51 N=mm2 Þ, em =sm according to Eq. (2); sm em P 0.6 Efss . a b 6.3 7.8 10.1 12.9 3.3 4.8 7.1 9.9 1.40 G3 151 182 227 284 7.6 9.1 11.4 14.2 80.2 80.2 80.2 80.2 5.9 7.7 10.2 13.3 0.12 0.15 0.20 0.27 4.5 5.5 6.8 9.6 0.13 0.16 0.20 0.28 0.10 0.12 0.16 0.21 0.09 0.15 0.22 0.27 0.15 0.19 0.26 0.33 0.20 0.24 0.30 0.38 5.7 7.2 9.5 12.4 1.6 3.2 5.5 8.3 0.94 G2 154 184 230 288 7.7 9.2 11.5 14.4 117.7 117.7 117.7 117.7 4.1 6.2 9.1 12.5 0.11 0.16 0.24 0.32 4.6 5.5 6.9 8.6 0.16 0.19 0.24 0.30 0.10 0.13 0.17 0.22 0.08 0.11 0.19 0.31 0.12 0.15 0.20 0.26 0.17 0.20 0.25 0.32 3.6 4.9 6.9 9.4 1.8 0.5 1.2 4.0 134 161 200 250 6.7 8.1 10.0 12.5 173.7 173.7 173.7 173.7 – 0.54 4.0 7.7 – 0.02 0.12 0.23 4.0 4.8 6.0 7.5 0.15 0.18 0.23 0.29 0.07 0.09 0.13 0.17 iii. 0.62 Wexperiments, (mm) fscr2 (N/mm2) esm · 104 Wk (mm) em · 104 em · 104 Wk (mm) em · 104 Wd (mm) Wmax (mm) Wmax (mm) Eurocode2-2001b fs (N/mm2) es = fs/Es · 104 Egyptian code 2007a l (%) 217 ii. G1 Table 3 Application of codes’ equations to beams tested by Makhlouf and Malhas  – Group B. BS 8110-97 ACI 318–95 Oh-Kang 1987 Measured crack width by Makhlouf and Malhas experiments Crack width evaluation for ﬂexural RC members iv. v. vi. (fs = 0.30 fy and fs = 0.37 fy). According to the Egyptian code, at steel stress fs = 0.30 fy (specimen G1), the section is considered uncracked. However, the values of crack width as proposed by the Egyptian code correlated well with the experimental values, at all levels of steel stress, for sections having percentage of reinforcement (l = 0.94%). On the other hand, for sections having higher percentage of reinforcement (l = 1.4%) the Egyptian code calculated crack width is lower than the crack width was measured experimentally. That may imply that a maximum reinforcement ratio for crack control should be determined. The underestimated values of crack width did not appear in Eurocode2 predictions at low levels of steel stress, since Eurocode2 limits the value of em not to be less than 0.6 fs/Es, as appears from Table 3. Table 3 gives the values of steel strain es together with the values of the average strain (esm or em). The results, obtained from both the Egyptian code and BS 8110, indicate that with the increase of reinforcement ratio l, the estimated concrete contribution in tension (tension stiffening) decreased. In general, the limitation of average strain introduced by Eurcode2 predicts realistic values of crack width than those predicted by the Egyptian code. In addition, with increase of the steel stress, the contribution of tensioned concrete decreased. Generally, the ACI 318-95 equation greatly overestimated the values of the crack width, except at high level of steel stress and at high values of reinforcement ratio (l = 1.4%). It should be noted that ACI 318-05 switched from the procedure of calculating the crack width and adopts a simpliﬁed equation for the maximum bar spacing. For values of steel stress 134–284 N/ mm2 (which are the levels of stress at which crack width were measured experimentally), equation 9 of ACI 31805 yields maximum permitted bar spacing of 625– 250 mm, for concrete clear cover = 50 mm. The values of crack width predicted using BS 8110-97 equations were smaller than the experimental values at high levels of steel stress. As given in Table 3, high values of mean strain em were proposed using BS 8110-97 and this indicates small contribution of tensioned concrete. The Oh-Kang  formula (Eq. (13)) correlated well with the experimental values of crack width for most specimens used in the comparison. 5.1.2. Effect of concrete cover, (c) The value of concrete cover may be considered as the second important factor that affecting the crack width, but its efﬁciency is considered in different ways in the building codes. Makhlouf and Malhas  reported results of tests on eight beams reinforced with high strength deformed bars as given by Fig. 2 and Table 2, Group ‘‘A’’. The maximum crack width was recorded at the reinforcement level. Four of the beams were with 22 mm concrete clear cover and the other four were with 52 mm concrete clear cover. The aim of these tests was to investigate the effect of increasing the concrete clear cover on the crack width. The results showed that a 16% increase in the crack width was obtained as a result of increasing the concrete cover. 218 S.M. Allam et al. Crack Width (mm) 0.40 0.35 ECP-2007 0.30 EuroCode2001 0.25 ACI 318-95 0.20 Oh and Kang  0.15 Experimental 0.10 B.S. 8110-97 0.05 0.00 100 150 200 250 300 Steel Stress (N/mm2 ) Figure 3 Crack width versus steel stress for G1 (l = 0.62%) Makhlouf and Malhas . Crack Width (mm) 0.40 0.35 ECP-2007 0.30 EuroCode2001 0.25 ACI 318-95 0.20 Oh and Kang  0.15 Experimantal 0.10 B.S. 8110-97 0.05 0.00 100 150 200 250 300 Steel Stress (N/mm2) Figure 4 Crack width versus steel stress for G2 (l = 0.94%) Makhlouf and Malhas . 0.40 Crack Width (mm) 0.35 ECP-2007 0.30 EuroCode2001 0.25 ACI 318-95 0.20 Oh and Kang  0.15 Experimental 0.10 B.S. 8110-97 0.05 0.00 100 150 200 250 300 Steel Stress (N/mm 2) Figure 5 Crack width versus steel stress for G3 (l = 1.40%) Makhlouf and Malhas . Table 4 gives and compares the values of the crack width calculated using the equations proposed by the building codes for the beams tested by Makhlouf and Malhas  and also, the equation developed by Oh and Kang . According to Oh and Kang , an increase of the crack width by about 20% is obtained with increase of the concrete cover from Crack width evaluation for ﬂexural RC members Table 4 219 Application of codes’ equations to beams tested by Makhlouf and Malhas  – Group A. Egyptian code 2007a Eurocode2-2001b BS 8110-97 ACI 318-95 Oh and Kang  fscr2 (N/mm ) esm · 10 Wk (mm) em · 104 em 104 Wk (mm) Wd (mm) Wmax (mm) Wmax (mm) GA11 GA21 251.2 287.44 2.9 – 0.06 – – 6.2 0.5 7.7 7.7 0.16 0.33 110.0% 0.12 0.14 20.0% 0.17 0.29 72.4% 0.19 0.23 17.9% GA12 GA22 144.5 165.36 9.5 8.5 0.17 0.23 35.5% 8.6 5.5 8.6 7.7 0.15 0.27 84.5% 0.14 0.19 32.1% 0.17 0.29 73.3% 0.21 0.25 19.2% GA13 GA23 94.4 108.1 11.4 10.9 0.18 0.25 40.6% 9.8 7.8 9.8 7.8 0.14 0.26 79.1% 0.15 0.20 38.5% 0.17 0.30 74.3% 0.22 0.27 20.6% GA14 GA24 61.9 70.9 12.1 12.0 0.17 0.24 38.6% 10.5 9.2 10.5 9.2 0.13 0.27 107.8% 0.14 0.20 45.4% 0.17 0.30 75.6% 0.24 0.29 22.4% 95.4% 34.0% 73.9% 20.0 2 Average increase in crack width 4 38.3% fs = 255.0 N/mm2, es = fs/Es = 12.75 · 104, – Uncracked section according to the Egyptian code. Bold values refer to the percentage of the increase of the crack width value in each two specimens, however italic values refer to the average increase in the crack width for all specimens in each column of the table. 22 mm to 52 mm. This amount of increase is very close to the value obtained experimentally by Makhlouf and Malhas . However, such increase in the values of crack width as predicted by the building codes was greatly overestimated as compared to the experimental results. The maximum percentage of increase was recorded by Eurocode2 followed by ACI 318-95 while the Egyptian code 2007 and BS 8110-97 give reasonable predictions. 6. Conclusions From the results obtained from the comparison of several building codes’ equations and from the theoretical work presented in this paper through studying the main variables affecting crack width, such as the concrete cover, steel stress, reinforcement ratio, bar surface, and reinforcement arrangement, the following conclusions may be drawn: 1. Values of crack width predicted by the code equations showed a large scatter among the different code equations and those obtained by other researchers. The Egyptian code equation predicted values very close to those predicted by ACI 318-95 and Eurocode2 equations except sections with low reinforcement ratio. For this case, the Egyptian code equation predicts values of crack width smaller than those predicted by ACI or Eurocode2. 2. Values of crack width, predicted using BS 8110-97, were less than those predicted by other building codes or by equations developed by researchers, especially for sections reinforced with plain mild steel bars. It should be noted that BS 8110 gives rules for bar detailing to ensure control of cracking rather than giving detailed calculations for crack width and crack spacing. 3. With the increase of reinforcement ratio l, the concrete contribution in tension decreases, the mean steel strain increases, consequently the crack width increases. However, for crack control, it is suggested to limit the reinforcement ratio instead of limiting the steel stress. 4. The reinforcement detailing (i.e. the bars distribution) is an important factor affecting crack width. With the well choice of bar arrangement (larger number, smaller diameter), better bond between concrete and steel occurs resulting in a reduction in the crack spacing. In addition to BS-8110 recommendations for crack control, ACI 318-05 switched for the procedure of calculating the crack width and adopts simpliﬁed equation for the maximum bar spacing. 5. The effect of bar surface deformation on the calculation of crack width not only affects the crack spacing, but also affects the mean strain. When the bond between the concrete and the steel increased, more tension force is transferred to the concrete between cracks. With the increase in the concrete contribution in tension, less slip between concrete and steel occurs, hence less value of total elongation between them; (i.e. esm ecm); and consequently resulting in less crack width. However, the effect of bar surface deformation is not considered in most codes’ formulas except the Egyptian code and Eurocode2. 6. Most equations proposed by the building codes overestimate the effect of the concrete cover on the calculated values of crack width when compared with the experimental results. However, Oh and Kang  formula, (Eq. (13), correlated well with the experimental values of crack width for most specimens used in the comparison. 7. The limitation of the average strain em not to be less than 0.6 fs/Es introduced by Eurocode2 results in realistic values of crack width when compared with experimental results than those predicted by the Egyptian code at low levels of steel stress for sections reinforced with low reinforcement ratios. 8. Comparison of building codes against experimental results revealed that the Egyptian code gives underestimated values of crack width for members reinforced with low reinforcement ratios especially at low level of steel stresses. The ECP 203-2007 adopted the use of mean strain similar to the equation given by Leonhardt . The Egyptian code equation expresses the tension stiffening as a function of the 220 steel stress. For the calculation of the steel stress just after the ﬁrst cracking, the Egyptian code assumes that the force resisted by concrete in tension is completely neglected immediately after the occurrence of the ﬁrst crack. This assumption produces a very large value of steel stress just after cracking (fscr2) for members having low reinforcement ratios especially, at low levels of steel stress. Values of fscr2 higher than fs indicate uncracked sections. It should be noted that by deﬁnition fscr2 should be less than fs. Therefore, for sections with low percentage of reinforcement, it is recommended, when using Eq. (5) of the ECP 2032007, to limit the value fscr2 to fs (the steel stress under working load conditions). References  A.S. Hassan, Crack Control for Reinforced Concrete Members Subjected to Flexure, M.Sc. Thesis, Alexandria University, Alexandria, Egypt, 2008, 119pp.  R. Saliger, High grade steel in reinforcement concrete, 2nd Congress, International Association for Bridges and Structural Engineering, Preliminary Publication, Berlin-Munich, 1936, pp. 293–315 (cited by MacGregor et al. (1980).  F.G. Tomas, Cracking in reinforced concrete, Structural Engineer 14 (7) (1936) 298–320 (cited by MacGregor et al. (1980).  B.B. Broms, Crack width and crack spacing in reinforced concrete members, Journal of American Concrete Institute 62 (10) (1965) 1237–1256.  G.D. Base, J.B. Read, A.W. Beeby, H.P.J. Taylor, An Investigation of the Crack Control Characteristics of Various Types of Bar in Reinforced Concrete Beams, Research Report No. 18, Parts I and II, Cement and Concrete Association, London, 1966 (cited by Nawy (1968)).  G.B. Welch, M.A. Janjua, Width and Spacing of Tensile Cracks in Reinforced Concrete, UNICIV Report No. R76, University of NSW, Kensington, 1971 (cited by Warner and Rangan (1977)).  F. Leonhardt, Crack Control in Concrete Structures, IABSE Surveys, No. S4/77, International Association for Bridges and Structural Engineering, Zurich, 1977, 26 pp (cited by Rizkalla (1984)).  P. Gergely, L.A. Lutz, Maximum Crack Width in RC Flexural Members, Causes, Mechanism and Control of Cracking in Concrete, SP-20, American Concrete Institute, Detroit, 1968, pp. 87–117.  B.h. Oh, Y.J. Kang, New formulas for maximum crack width and crack spacing in reinforced concrete ﬂexural members, ACI Structural Journal 84 (2) (1987) 103–112.  R.J. Frosch, Another look at cracking and crack control in reinforced concrete, ACI Structural Journal 96 (3) (1999) 437– 442.  M.H. Makhlouf, F.A. Malhas, The effect of thick concrete cover on the maximum ﬂexural crack width under service load, ACI Structural Journal 93 (3) (1996) 257–265. View publication stats S.M. Allam et al.  A.W. Beeby, Prediction and Control of Flexural Cracking in Reinforced Concrete Members, Cracking, Deﬂection and Ultimate Load of Concrete Slab System, SP-20, American Concrete Institute, Detroit, 1971, pp. 55–75 (cited by Makhlouf and Malhas (1996)).  E.G. Nawy, K.W. Blair, Further Studies on Flexural Crack Control in Structural Slab Systems, Cracking, Deﬂection, and Ultimate Load of concrete Slab Systems, SP-20, American Concrete Institute, Detroit, 1971, pp. 1–42.  R.I. Gilbert, S. Nejadi, An Experimental Study of Flexural Cracking of Reinforced Concrete Members under Sustained Loads, UNICIV Report No. R-435, School of Civil and Environmental Engineering, University of New South Wales, Sydney, Australia, 2004, 59pp (cited by Gilbert (2008)).  Eurocode 2: Design of Concrete Structures – Part 1: General Rules and Rules for Buildings 1992-1, European Committee for Standardization, October 2001, Belgium.  The Egyptian Code for Design and Construction of Reinforced Concrete Structures, ECP 203-2007, Ministry of Housing, Egypt.  Building Code Requirements for Reinforced Concrete, ACI 31895 and Commentary ACI 318R-95, American Concrete Institute, Detroit, 1995.  Concrete sanitary engineering structures, a report by ACI committee 350, ACI Structural Journal 80 (1983) 467–486.  A.W. Beeby, Corrosion of reinforcing steel in concrete and its relation to cracking, Structural Engineer 56A (3) (1978) 77–81.  A.W. Beeby, Cracking, cover, and corrosion of reinforcement, Concrete International Design and Construction 5 (2) (1983) 35– 40.  Building Code Requirements for Reinforced Concrete, ACI 31805 and Commentary ACI 318R-05, American Concrete Institute, Detroit, 2005.  Building Code Requirements for Reinforced Concrete, ACI 31808 and Commentary ACI 318R-08, American Concrete Institute, Detroit, 2008.  Structural Use of Concrete, Part 2: Code of Practice for Special Circumstances BS 8110: Part 2: 1997, British Standard Institution, London, 1998.  E. Hognestad, High strength bars as concrete reinforcement – Part 2: Control of ﬂexural cracking, Journal Portland Cement Association Research and Development Laboratories 4 (1) (1962) 46–63 (cited by Park and Paulay (1975)).  P.H. Karr, A.H. Mattock, High-strength bars as concrete reinforcement – Part 4: Control of cracks, Journal of the PCA Research Development Laboratories 5 (1) (1963) 15–38 (cited by Park and Paulay (1975)).  P.H. Karr, E. Hognestad, High-strength bars as concrete reinforcement – Part 7: Control of cracks in T-beams ﬂanges, Journal of the PCA Research Development Laboratories 7 (1) (1965) 42–53 (cited by Park and Paulay (1975)).  A.P. Clark, Cracking in reinforced concrete ﬂexural members, ACI Structural Journal 27 (8) (1956) 851–862 (cited by Frosch (1999) and Oh-Kang (1987)).  H. Rusch, G. Rehm, Versuche mit Beton formstahlen, Deutscher Ausschuss fur Stahlbcton, bulletins, No. 140, Part I, 1963. No. 160 Part 2, 1963; and No. 165, Part 3, 1904 (cited by Frosch (1999)).